Advanced Gas Turbine
Materials and Coatings
efficiencies as high as 60% are now achievable because of
increased firing temperature coupled with more efficient component and
This paper describes the evolution of solutions to what used to be incompatible
market demands: high firing temperatures and long life, corrosion protection
from contaminated fuels and air, and higher efficiency with fuel flexibility. It
concentrates on advances made in the hot gas path components because they
are generally the most critical part of the gas turbine.
Improvements in superalloys and processing now permit the hot gas path
components to operate in advanced gas turbines firing at increased
temperatures for many thousands of hours under severe conditions of
centrifugal, thermal and vibratory stresses. Recent improvements to
compressors and rotors are also discussed.
2. Turbine Buckets and Nozzles
GE has used investment cast nozzles and buckets made by the lost wax
technique since the mid-1960s. This casting process allows the use of alloys that
are difficult to form or machine and provides great design flexibility for internal
cooling schemes. For example, ceramic coring is used extensively in these
castings to form air-cooling passages and to provide weight reduction.
Most nozzle and bucket castings used by GE are made by using the
conventional equiaxed investment casting process. In this process, the molten
metal is poured into a ceramic mold at a pressure below 10-2 torr (10-2 mm
Hg). Vacuum is used in most cases, except for some of the cobalt alloys, to
prevent the highly reactive elements in the superalloys from reacting with the
oxygen and nitrogen in the air. With proper control of metal and mold thermal
2. conditions, the molten metal then solidifies from the surface toward the center
of the mold, creating an equiaxed structure. To pre
Directional solidification (DS) is also being employed to produce advanced
3. 2.2 Bucket Materials
The stage 1 bucket must withstand the most severe combination of
temperature, stress and environment; it is generally the limiting component in
Since 1950, turbine bucket material temperature capability has advanced
approximately 850°F/472°C, approximately 20°F/10°C per year. The
importance of this increase can be appreciated by noting that an increase of
100°F/56°C in turbine firing temperature can provide a corresponding increase
of 8% to 13% in output and 2% to 4% improvement in simple-cycle efficiency.
Advances in alloys and processing, while expensive and time-consuming,
provide significant incentives through increased power density and improved
Figure 4 shows the trend of firing temperature and bucket alloy capability. The
composition of the new and conventional alloys discussed is shown in Table 1.
The increases in bucket alloy temperature capability accounted for the majority
of the firing temperature increase until the 1970s, when air cooling was
introduced, which decoupled firing temperature from bucket metal
temperature. Also, as the metal temperatures approached the 1600°F/870°C
range, hot corrosion of buckets became more life-limiting than strength until
the introduction of protective coatings.
During the 1980s, emphasis turned toward two major areas: improved
processing to achieve greater bucket alloy capability without sacrificing alloy
corrosion resistance; and advanced highly sophisticated air-cooling technology
to achieve the firing temperature capability required for the new F generation of
gas turbines. (See Figure 5.) The use of steam cooling to further increase
combined-cycle efficiencies will be realized in the 1990s.
All GE gas turbine bucket alloys are vacuum cast, nickel-base superalloys that
are strengthened through solution and precipitation-hardening heat treatments.
Figure 6 shows the stress rupture strength of these alloys and the superalloys
used for nozzle applications: GTD-222, FSX-414 and N-155. This comparison
is presented in the form of the stress required for rupture as a function of a
4. parameter that relates time and temperature (the Larson- Miller Parameter).
This parameter is one of several important design parameters that must be
satisfied to ensure proper performance of the alloy in a bucket application,
especially for long service life. Creep life, high- and low-cycle fatigue, thermal
fatigue, tensile strength and ductility,
5. 2.3. Bucket Coatings
Bucket coatings are required to protect the bucket from corrosion, oxidation
and mechanical property degradation. As superalloys have become more
complex, it has been increasingly difficult to obtain both the higher strength
levels that are required and a satisfactory level of corrosion and oxidation
resistance without the use of coatings. Thus, the trend toward higher firing
temperatures increases the need for coatings. The function of all coatings is to
provide a surface reservoir of elements that nwill form very protective and
adherent oxide layers, thus protecting the underlying base material from
oxidation and corrosion attack and degradation. Experience has shown that the
lives of both uncoated and coated buckets depend to a large degree on the
amount of fuel and air contamination, as well as the operating temperature of
the bucket. This effect is shown in Figure 10, which illustrates the effect of
sodium, a common contaminant, on bucket life at 1600°F/871°C. The
presence of increased levels of contaminants give rise to an accelerated form of
attack called hot corrosion. In addition to hot corrosion, high-temperature
oxidation and thermal fatigue resistance have become important criteria in the
gas turbines, as shown in Figure 11. In today’s advanced machines, oxidation is
of concern not only for external buckets surfaces, but also for internal passages
such as cooling holes.
6. 2.4. Hot Corrosion
Hot corrosion is a rapid form of attack that is generally associated with alkali
metal contaminants, such as sodium and potassium, reacting with sulfur in the
fuel to form molten sulfates.
Presence of only a few parts per million (ppm) of such contaminants in the
fuel, or equivalent in the air, is sufficient to cause this corrosion. Sodium can be
introduced in a number of ways, such as salt water in liquid fuel, through the
turbine air inlet at sites near salt water or other contaminated areas, or as
contaminants in water/steam injections.
Besides the alkali metals such as sodium and potassium, other chemical
elements can influence or cause corrosion on bucketing. Notable in this
connection are vanadium, primarily found in crude and residual oils, and lead,
most frequently resulting automobile exhaust emissions or as transportation
contaminate from leaded gasoline.
There are now two distinct forms of hot corrosion recognized by the industry,
although the end result is the same. These two types are high-temperature
(Type 1) and low-temperature (Type 2) hot corrosion.
7. 2.4. High-Temperature Oxidation
Metal oxidation occurs when oxygen atoms combine with metal atoms to form
oxide scales. The higher the temperature, the more rapidly this process takes
place, creating the potential for failure of the component if too much of the
substrate material is consumed in the formation of these oxides. Figure 14a
shows the microstructure of a coated bucket that has seen about 30,000 hours
of service. At the temperatures seen in this region of the airfoil, no significant
oxidation attack of the coating can be seen.
By contrast, Figure 14b shows the microstructure of the same type of coating,
which has been severely attacked after about the same length of service. At the
8. 2.5 High-Temperature Coatings
High-temperature coatings are used where the temperatures of the components
exceed the inherent oxidation resistance of the material. Considerable
development has occurred during the past 20 years in the field of high
temperature coatings. The result has been a marked increase in the capability of
these coatings to resist not only hot corrosion attack over long periods of time,
but high-temperature oxidation as well. GE heavy-duty coatings avail-able
today have lives that are 10 to 20 times longer than the first-generation coatings
under a wider diversity of corrosion and oxidizing conditions.
GE has used two basic classes of coatings during the past 25 years.
The first class used was a diffusion- style coating called platinum aluminide
(PtAl). The second class is an overlay-style coating such as
PLASMAGUARD™ GT-29 INPLUS ™.